# Dynamic Characterisation of Honeycomb CNT Reinforced Sandwich Composite Structure

←

→

**Page content transcription**

If your browser does not render page correctly, please read the page content below

Journal of Physics: Conference Series PAPER • OPEN ACCESS Dynamic Characterisation of Honeycomb CNT Reinforced Sandwich Composite Structure To cite this article: S Balaji et al 2021 J. Phys.: Conf. Ser. 1969 012016 View the article online for updates and enhancements. This content was downloaded from IP address 46.4.80.155 on 13/09/2021 at 14:49

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 Dynamic Characterisation of Honeycomb CNT Reinforced Sandwich Composite Structure Balaji S1; Abhishek K Nanavate 2, Lakshmi Pathi Jakkamputi 3,*, Raghukiran N4 and Jegadeeshwaran R5 1,2,3,5 School of Mechanical Engineering, Vellore Institute of Technology, Chennai, India. 4 Centre for Automation, Vellore Institute of Technology, Chennai, India Email id 1 : balaji.s2020a@vitstudent.ac.in *Corresponding author : lakshmipathi@vit.ac.in Abstract. The dynamic characterization of honeycomb sandwich structure with CNT reinforced hybrid composite face sheet is performed using Finite element simulation. The element simulations. The Potential and Kinetic energies of the honeycomb sandwich beam were derived using classical laminate beam theory and Mindlin theory. The governing equations of motion for the sandwich composite beam is made up of Nomex material with a hybrid composite face sheet reinforced with CNT are obtained by applying the Hamilton rule in the finite element model. The functionality of current finite element modeling has been investigated to proving the dynamic properties acquired from the improved finite element model with the solution obtainable in the previous literature. A further various parametric study is performed to understand the effect of CNT content, thickness ratio, and boundary constraints on the honeycomb sandwich composition of dynamic properties with reinforced CNT of the hybrid composite face sheet is performed using finite element simulation. The CNT content in the honeycomb sandwich beam containing a remarkable effect on the natural frequency. Keywords. Honeycomb sandwich structure, CNT reinforced composite beam, model analysis, dynamic characteristic. 1. Introduction From recent decades, Engineering construction is excepting for lightweight materials with high stiffness and low-density properties. Other Important properties which are expected are to be present are large energy-absorbing capacity and tolerances to damage. To acquire these properties every industry is opting for composite materials and lightweight structures. The integration of two or multiple materials with various physical along with chemical properties categorized as a composite material. There are many types of composite materials available which has large energy absorbing capacity and damage tolerances. The one such composite material which is used is a combination of CNT epoxy glass Fiber- reinforced faced sheets and Honeycomb core with Nomex material. The tensile and compressive Loads are primarily carried by face sheets and these face sheets are supported by the core which is the Nomex honeycomb core to avoid resistance out of the plane shear load and buckling. Honeycomb windmill blades, helicopter blades, Automobile Industries, Satellites, Aircraft, marines, and bridge constructions, these composite sandwich structures are used. Nomex honeycomb core which is manufactured by aramid paper saturated is bionic material which is produced using poly fiber paper (m-phenylene isophthalamide) [1] with heat-resistant phenolic resin and this Nomex honeycomb core is a non-metallic product combination of superior electrical insulation good resilience and absorbent to shocks. In this study, the core of the honeycomb is processed as an orthotropic uniform material. The design of honeycomb structure using finite element method to acquire the natural mechanical characteristics of the honeycomb sandwich composition [2]. The studies related to Nomex honeycomb have increased in Content from this work may be used under the terms of the Creative Commons Attribution 3.0 licence. Any further distribution of this work must maintain attribution to the author(s) and the title of the work, journal citation and DOI. Published under licence by IOP Publishing Ltd 1

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 the recent decades. However, the properties for outer plane shear are reliant on properties with core geometry as well as material for Nomex honeycomb. In order to attain the required corresponding elastic limits of the structure of the Nomex honeycomb is the finite element (FE) model is formed. The whole geometrical property of the honeycomb is not considered because the cost of computation will be more. In engineering applications where rotating composites are found such as windmill rotor blades, turbine blades helicopter tail, and main blades, there exist adverse vibrations to the structure due to high levels of dynamic loads. The improvised mechanical characteristics can be achieved to the matrix by the addition of a small amount of multiple walled carbon nanotubes (MWCNT) was acknowledged by various literature work. Further, these studies show the comparison between CNT-Reinforced polymer rotating structures and carbon-fiber-reinforced where CNT-Reinforced structure showed great dynamic performance compared to the latter [3]. The effect of CNTs proportion is set up to be more clear in nonrotatable structures instead of the rotatable structures because of enhancing the CNT-FRP nanohybrid composites of dynamic properties. The primary natural frequency of rotatable CNT reinforced nanocomposites is enhanced almost by 5% while present angular speed varies from o to 500 rpm [4]. The dynamic performance of CNT -reinforced hybrid composite is studied in which also explains the dynamic instability features for main and subsidiary rotatable CNT- reinforced non-uniform composite plates [5]. Various studies and experiments have been conducted on CNTRC which influenced the uses in different fields of engineering. The reinforcement of CNT face sheets of a sandwich plate having the thickness ratio and CNT volume fraction causes instability in width. The sections of dynamic instability of laminated composites are determined using Higher-order shear deformation theory [6]. However, the rotatable fiber-reinforced laminated composites considerably control the design principles about stability properties by entrenching MWCNT is appreciable. The potential, as well as kinetic energy equations, are derived using Mindlin and Reissner also called First-order shear deformation (FSDT). The governing equation of motions was calculated using the Hamilton rule. To obtain outstanding elastic properties, as well as damping properties effectively by adding a small amount of CNT will improve the vibrational characteristics of CNT- based composite structure. Several research works suggested that to produce good mechanical properties containing the dynamic characteristics of the structures by combining CNT into stationing the composite matrix and in addition because of slippage among inner and exterior graphene plies of a composite structure having damping properties of MWCNT with enhanced stiffness. At higher frequencies, from 0 to 2 % CNT volume fractions were raising incrementally because of the source of dynamic instability [7]. The sandwich plate having increasing core thickness will increase the natural frequencies. The comparison in mode shape for a minimal three vibration of the sandwich plate was noted with an enhanced CNT which presents the potency of CNT in honeycomb sandwich plate which reduces the vibrational amplitude [9]. The various parametric studies were also carried out in the CNT composite plate to examine the result of CNT volume fractions and static load factors on the region for dynamic instability. 2. Numerical representation of CNT reinforced Nomex honeycomb composite beam. 2.1. Kinematics of Euler Beam • The transverse normal perpendicular to the midplane of the beam remains straight and perpendicular even after deformation. • The transverse normal does not undergo any extension. 2

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 Figure 1. Euler Beam representation with planes. Figure 2. Before and After deformation of the midplane and transverse plane. The shear strain is zero and the angle between the midplane and transverse normal after bending is 90o ∵ γxz =0 ∂u ∂w + =0 ∂z ∂x Where u and w are deformation and deflection along x and z direction respectively. ∂u ∂w - =0 ∂z ∂x Assuming z=0 (i.e Midplane of the beam) and u= u0 (i.e Midplane deformation along x - direction ) ∂w ∴ u= u0 - z (1) ∂x Transverse normal is not undergoing any deformation. So, ∵ εzz =0 ∂w =0 ∂z Assuming z = 0 (i.e Midplane of the beam) and w= w0 (i.e Midplane deflection ). w=w0 3

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 2.1.1 Strain field in the Beam ∂u εx = (2) ∂x From equation (1), ∂u0 ∂2 w0 εx = -z (3) ∂x ∂x 2.1.2 Stress field in the Beam σx = Eεx From equation (3), ∂u0 ∂2 w0 σx =E { -z } (4) ∂x ∂x Figure 3. Force and moment per unit length of the sheet. Nx = ∫ σx dz Mx = ∫ Z σx dz Where Nx and Mx are force acting per unit length and moment acting per unit length. Nx = ∫ σx dz From equation (4), We know that σ = Q(ε0 + z ) (5) Where Q = E 4

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 Midplane strain ∂u0 ε0 = (6) ∂u Midplane curvature −∂2 w0 Kx = (7) ∂x2 Nx = ∫ Qε0 dz + ∫ QZ Kx dz (8) Mx = ∫ Zσx dz (9) Representing the midpane strain and curvature ε0 (10) Nx A B ∴ { } = [ ] { } Mx B D Kx N zt N A = ∑ ∫ Q dz = ∑ Q (Zt - Zb) (11) i = 1 zb i=1 N zt N Q 2 B = ∑ ∫ Q z dz = ∑ (Zt - Zb2 ) (12) 2 i = 1 zb i=1 N zt N Q 3 D = ∑ ∫ Q z dz = ∑ 2 (Zt - Zb3 ) (13) 4 i = 1 zb i=1 Figure 4. Interpretation of sandwich structure with thickness of beam 2.1.3 Strain energy due to midplane strain and curvature 1 U= ∫ Nx dy ε0 dx + Mx dy Kx dx (14) 2 5

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 2.1.4 Kinetic energy 1 T= ∫ ρ vT v dv (15) 2 Where u̇ v= { } (16) ẇ Therefore, u0̇ T u0̇ 1 IT 0 IC ẇ ẇ0 T = ∫{ 0 } [0 IT 0]{ } dx (17) 2 ∂ẇ ∂ẇ - IC 0 IR - ∂x ∂x 2.2. Kinematics of sandwich beam Figure 5. Nomex Honeycomb with CNT reinforced Figure 6. Assembled image Sandwich Composite sandwich layers structure 2.2.1 Assumptions • No slippage was assumed between the face sheets and sandwich core • All three layers experience the same transverse deflection • The normal stresses are negligible in the sandwich core as compared with the face sheets • Rotary inertia effects are negligible • No shear strain in the face sheets 6

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 Figure 7. Depiction of layers of sandwich composite Figure 8. Mid-plane deformation of layers structure ∂u ∂w γxz = + (18) ∂z ∂x h1 2 Nx1 = ∫ Q( ε0 + z Kx )dz (19) h - 1 2 h1 2 Nx2 = ∫ Q( ε0 + z Kx )dz (20) h - 3 2 Then, ∂u ∂w γxz = + ∂z ∂x u01 - u03 h ∂w γxz = + (21) h2 h2 ∂x u01 + u03 h1 - h3 ∂w u02 = + (22) 2 4 ∂x where u01 , u02 and u03 are the midplane deformation of layer 1, layer 2, and layer 3 respectively. 7

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 Figure 9. Representation of force and moment action per unit length with for two facesheets. h1 2 Nx1 = ∫ σx dz (23) h - 1 2 h3 2 Nx2 = ∫ σx dz (24) h - 3 2 h1 2 Mx1 = ∫ Z σx dz (25) h - 1 2 h3 2 Mx2 = ∫ Z σx dz (26) h - 3 2 h2 1 2 T2 = ∫ z2 ρ γ̇ 2 xz dx dy dz 2 h2 2 By solving the above expression, we get, 1 u0̇ - u0̇ 3 h ∂ẇ u0̇ - u0̇ 3 h ∂ẇ (27) T2 = w {{ 1 } + } [Iγ2 ] {{ 1 } + } 2 h2 h2 ∂x h2 h2 ∂x Here, T1 = Translation kinetic energy of the three layered Beam T2 = Rotational kinetic energy of the sandwich core 8

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 2.3. Finite element formulation u01 = N1 u01 + N2 u01 (28) 1 2 u03 = N1 u03 + N2 u03 (29) 1 2 w0 = Nw1 w01 +Nθ1 wθ1 + Nw2 w02 +Nθ2 wθ2 (30) u01 N1 0 0 0 N2 0 0 0 u { 03 } = [ 0 N1 0 0 0 N2 0 0 ] (31) w0 0 0 Nw1 Nθ1 0 0 Nw2 Nθ2 Figure 10. Element formulation 2.3.1 Strain energy 1 U= ∫ Nx1 dy ε01 dx + ∫ Nx2 dy ε02 dx + ∫ Mx dy Kx dx 2 ε01 T Nx1 1 U = 2 ∫ W {ε02 } {Nx2 } dx (32) Kx Mx 2.3.2 Kinetic energy 1 T= 2 ∫ ρ VT V dv (33) ∂ẇ u0̇ 1 u̇ 01 - Z ∂x V= {u0̇ 3 } = ∂ẇ (34) u̇ 03 - Z ẇ ∂x { ẇ } 9

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 u0 1 1 ∂u01 u0 3 1 ∂x w01 N11 x 0 0 0 N21 x 0 0 0 ∂u03 θ = [ 0 N11 x 0 0 0 N21 x 0 0 ] u1 ∂x -Nw22 xx -Nθ22 xx 012 2 0 0 -Nw11 xx -Nθ11 xx 0 0 u ∂ w 031 - { ∂x2 } w 02 { θ2 } ∂u01 ∂x ∂u03 = [B]{d} (35) ∂x ∂2 w {- ∂x2 } u̇ 01 1 u̇ 03 1 u̇ 01 ẇ 01 N1 0 0 0 N2 0 0 0 u̇ 03 N1 0 0 N2 0 0 θ̇ 1 ẇ = [0 N N 0 N N ] 0 0 w 1 θ1 0 0 w 2 θ2 u̇ 01 ∂ẇ 2 0 0 -Nw11 x - Nθ11 x 0 0 -Nw21 x - Nθ21 x u̇ 03 { ∂x } 1 ẇ 02 { θ̇ 2 } u̇ 01 u̇ 03 ẇ = [N] {ḋ } (36) ∂ẇ { ∂x } u0̇ 1 - u̇ 03 h ∂ẇ 1 + = [N1 -N1 Nw11 x hNw1 x N2 -N2 Nw21 x hNθ21 x]{d} h2 h2 ∂x h2 u0̇ 1 - u̇ 03 h ∂ẇ + ̇ = [N2 ]{d} (37) h2 h2 ∂x 2.3.3 Strain energy 1 U= ∫ w {d}T [B]T [ABD] [B]{d}dx (38) 2 1 U= {d}T [Kel ] {d} 2 10

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 2.3.4 Kinetic energy 1 T T1 = 2 ∫ w {del̇ } [N1]T [I][N1 ]{ ḋ el }dx (39) 1 T T2 = 2 ∫ w {del̇ } [N2]T [Iγ2 ][N2 ]{ ḋ el }dx (40) T = T1 + T2 (41) After Assembly, 1 U= {d}T [K] {d} (42) 2 1 T T = {ḋ } [M]{ ḋ } (43) 2 Lagrange , L=T-U (44) From lagrange Equation, d ∂L ∂L - ( ) + ( ) =0 (45) dt ∂q̇ i ∂qi Hence we can obtain, [M]{d̈ }+ [k]{d} = 0 (46) 3. Affirmation of finite element formulations The dynamic properties were evaluated for the Nomex honeycomb core with CNT composite plates and to validate the Finite element model through performed MATLAB simulation. Table 1. material properties of Nomex Honeycomb Structure [3]. Parameter Value E1 5000 Mpa E2 4000Mpa G12 1250Mpa μ 0.3 ρ 48 kg/ 3 11

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 Table 2. Material properties of CNT Name of the material Literature reference Indication Numerical Value Description Ecn2 11 640000 Mpa Modulus of elasticity of CNT Ecn2 22 10000 Mpa Modulus of elasticity of CNT Gcn2 12 17000Mpa Modulus of rigidity of CNT ρcn2 1350.0 Kg/ 3 Mass per unit volume of CNT CNT [10] vcn2 0.33 Poisson’s ratio of CNT tcn2 0.34nm The thickness of CNT dcn2 1.4nm The diameter of CNT lcn2 25 m Length of CNT Table 3. Material properties of Epoxy glass fiber Name of the material Literature reference Indication Numerical Value Description Ef 69000 Mpa Modulus of elasticity of E- glass fiber ν 0.2 Modulus of E- glass fiber [10] elasticity of E- glass fiber ρf 1200 Kg/ 3 Length of E- glass fiber 12

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 4. Parametric study: The dynamic characteristics of Nomex honeycomb reinforced with CNT epoxy fiber composite structure are effected by the material properties and the geometry of the structures. The effects can also influenced further by the composition of structures , variation of CNT weight percentage, varying thickness ratios. To understand the effects of these parameters on Nomex Honeycomb with CNT reinforced with CNT epoxy glass fiber, a parametric study is conducted. The orientation of composite beam ply is taken to [0o/90o] by considering an uniform configuration of the structure for geometrical dimensions length(L) 250 mm, Width (B) 25mm, thickness of lamina is 0.025 mm. The effects on composite beam are studied based on clamped- free and clamped-clamped end conditions. The required material properties of Nomex honeycomb structure along with CNT epoxy glass fiber are presented in the Table 1-3, to serve for the purpose of numerical calculations. The weightage percentage of CNT epoxy glass fiber composite is taken to be 0.0 and 1.0 and the thickness ratio (t\tc) to be taken as 2 for both boundary conditions. 4.1 Effect on natural frequency due to variation in weight percentage of CNT The variation of weightage percentage of CNT from 0 to 2.0% is considered to study the effect of natural frequency on uniform configuration of composite structure for clamped-free and clamped- clamped conditions.The outcomes pertaining to the effect are shown in Table 4 and Table 5. The increase in weightage percentage of CNT from 0 to 2% with ply orientation of [0o/90o], increase the natural frequencies for all nodes.This can be interpreted with fact that matrix of CNT used in epoxy glass fiber confines the movement of chain of polymers which ameliorate the strength and stiffness of the composite structure The trend can be seen when comparison is done between both of the end conditions ,there is an increase in values of natural frequency with the increase in mode shapes which exhibits that there is an improve in the stability of the structure. Table 4. Effect of natural frequency for cantilever beam by varying weightage percentage of CNT. End conditions for Beams modes The weight percentage of CNT m n 0.0 0.5 1.0 1.5 2.0 1 1 20.4 24.6 25.6 26.5 27.5 1 2 273.3 286.5 292.5 298.1 303.4 Clamped - free 1 3 864.1 893.7 910.0 929.2 945.3 1 4 1152.2 1360.1 1417.4 1473.4 1528.2 1 5 1531.4 1567.9 1590.4 1610.9 1629.8 13

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 Figure 11. First five-mode shapes for a clamped-free condition Figure 12. First five-mode shapes for a clamped-free with 0.0 weight percentage of CNT condition with 1.0 weight percentage of CNT. Table 5. Effect of natural frequency for fixed beam by varying weightage percentage of CNT. End conditions for Beams modes The weight percentage of CNT m n 0.0 0.5 1.0 1.5 2.0 1 1 33.4 34.2 34.9 35.56 36.17 1 2 812.7 826.3 838.7 850.2 860.8 Clamped - clamped 1 3 1425.2 1444.5 1461.9 1477.8 1492.6 1 4 2085.7 2107.4 2126.7 2144.4 2160.6 1 5 2771.7 2794.6 2815.0 2833.6 2850.9 Figure 13. First five-mode shapes for a clamped-clamped Figure 14. First five-mode shapes for a clamped-clamped condition with 0.0 weight percentage of CNT condition with 1.0 weight percentage of CNT. 14

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 4.2 Effect on natural frequency due to variation in weight percentage of CNT with change in thickness ratio The change in thickness ratio has shown significant improvement of increase in natural frequencies for uniform configuration of composite structure with ply oreientation of [0o/90o] along with increase in weight percentage of CNT from to 2.0% for increase in mode shapes. These variations are presented in Table 6 and Table 7 for both clamped-free and clamped-clamped conditions of composite beam. There is considerably increase in values of natural frequency in fixed condition of beam compared to cantilever type. This also results in improved dynamic properties of the composite structures. Table 6. Natural frequency for a clamped-free beam of Thickness ratio (t/tc )=2 with varying weightage percentage of CNT. End conditions for modes The weight percentage of CNT Beams m n 0.0 0.5 1.0 1.5 2.0 1 1 19.8 20.6 21.5 22.3 23.1 1 2 247.5 253.9 259.9 265.4 270.6 Clamped - free 1 3 775.9 794.6 811.9 828.2 843.5 1 4 1301.0 1360.1 1417.4 1460.8 1480.1 1 5 1392.3 1417.2 1439.9 1473.4 1528.2 Figure 15. First five-mode shapes for a clamped-free beam Figure 16. First five-mode shapes for a clamped-free by by applying thickness ratio (t/tc )=2 with 0.0 weight applying thickness ratio (t/tc )=2 with 1.0 weight percentage percentage of CNT. of CNT. 15

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 Table 7. Natural frequency for a clamped-clamped beam of Thickness ratio (t/tc )=2 with varying weightage percentage of CNT. End conditions for Beams modes The weight percentage of CNT m n 0.0 0.5 1.0 1.5 2.0 1 1 295.9 303.3 310.2 316.5 322.5 1 2 732.3 745.9 758.3 769.7 780.4 Clamped - clamped 1 3 1296.7 1316.2 1334.0 1350.2 1365.3 1 4 1916.1 1938.8 1959.1 1977.8 1994.9 1 5 2566.4 2590.9 2612.8 2632.9 2651.5 Figure 17. First five-mode shapes for a clamped-clamped Figure 18. First five-mode shapes for a clamped-clamped beam by applying thickness ratio (t/tc )=2 with 0.0 weight beam by applying thickness ratio (t/tc )=2 with 1.0 weight percentage of CNT. percentage of CNT. 5. Conclusion. In this study, based on FSDT theory we have evaluated the dynamic analysis for MWCNT composite with Nomex honeycomb core considering a cantilever beam. The Mori- Tanaka method and modified model of Hapin- Tsai helps to assess the elastic properties. Using FSDT the governing differential equation of motion for CNT Epoxy Glass Fiber which is derived in Finite element formulation. The amount of CNT add incrementally is an important parameter considering to evaluate the natural frequencies and also by varying the aspect ratio of thickness for core and composite fiber layers. Finally, the observation of this study explains that more dynamic stability will occur when incrementation of the aspect ratio of thickness for honeycomb core and composite e- glass fiber layers and also by adding a small amount of CNT from 0 to 2 weight percentage in the Nomex honeycomb sandwich structure. 16

IRMAS 2021 IOP Publishing Journal of Physics: Conference Series 1969 (2021) 012016 doi:10.1088/1742-6596/1969/1/012016 References: [1] Suchao X, Hao W, Chengxing Y, Hui Z and Zhejun F 2020 Mechanical properties of combined structures of stacked multilayer Nomex honeycombs J. Thin-Walled Structure 151 106729 p 01-12. [2] Yue L, Weicheng G, Wei L and Zhou H 2017 Numerical analysis and mechanical properties of Nomex Honeycomb core, IMECE 72654. [3] Yue L, Wei L and Weicheng G 2020 Out-of-plane shear property analysis of Nomex honeycomb sandwich structure J. Reinforced Plastics and Composites 0(0) p 1–11. [4] Deepak B. P, Ganguli R and Gopalakrishnan 2012 Dynamics of rotating composite beams: A comparative study between CNT reinforced polymer composite beams and laminated composite beams using spectral finite elements Int. J. Mech. Sci. 64 p 110–126. [5] Glaz B, Riddick J, Habtour E and Kang H, Interfacial strain energy dissipation in hybrid nanocomposite beams under axial strain elds AIAA J. 53(6), p 1544-54. [6] Lakshmipathi J, Rajamohan V and Sameer S. R 2019 Primary and secondary instability region analysis of rotating carbon nanotube–reinforced non-uniform, hybrid composite plates Int. J. Structural Stability and Dynamics 19(10) 1950115 p 01-33. [7] Sankar A, Natarajan S and Ganapathi M 2016 Dynamic instability analysis of sandwich plates with CNT reinforced face sheets, J. Compos. Struct. 146 p.187–200. [8] Lakshmipathi J and Rajamohan V 2019 Numerical investigation of dynamic instability of a rotating CNT reinforced composite plate, AIP Conference Proceedings 2057, 020003. [9] Lakshmipathi J and Rajamohan V 2018 Dynamic characterization of a CNT reinforced hybrid uniform and non- uniform composite plates 301. [10] Sang Y L 2018 Dynamic instability assessment of carbon nanotube/fiber/polymer multiscale composite skew plates with delamination based on HSDT J. Composite Structures 200 p 757– 70. [11] Paul P. A, Moheez M. A, Manjunath M. M, Ananda babu A and Vasudevan R 2019 Evaluation of shear properties of carbon nanotube reinforced functionally graded honeycomb composite materials”, AIP Conference Proceedings 2057, 020067. 17

You can also read